Morphological, Rheological and Mechanical Properties of Pla-Typha Based Biocomposites

Due to the demand from society for the consumption of ecological polymeric materials, one of the polymers that have satisfied this request is the poly (lactic acid) (PLA). This polymer is derived from renewable resources, it is recyclable and biodegradable. It presents a good understanding between the promising properties and the cost. However, a route to increase the mechanical properties and reduce the cost of PLA is the elaboration of PLA based biocomposites by using fillers from natural waste. In this work, The effect of Typha content on the morphological, rheological, thermal and mechanical properties of PLA matrix was studied. Four formulations were produced with different mass concentrations. The results showed an increase in the viscoelastic properties, as a function of the Typha stem powder concentration. The DSC analysis showed an increase in the crystallinity rate of the various composites confirming the nucleating effect provided by the filler. TGA analysis indicated a decrease in the decomposition temperature of the composites. Mechanical tensile tests have shown a significant improvement in the mechanical properties mainly for the samples containing 45% (w/w) of Typha powder.

on the part of plastic manufacturing companies [1]. The main advantage of using WPC composites is a reduction in the cost of final products. In addition to their biodegradability, they have other important properties, such as high specific stiffness, low density, renewal capacity [2] [3] [4]. Furthermore, an increasingly important interest takes into consideration the aesthetic values of these composites. In fact, the products made with a composite having a large fraction of fillers have an appreciated appearance of the surface and particular sensation to the touch. This characteristic distinguishes them compared to traditional polymers. At the same time, due to their much higher resistance to atmospheric factors compared to wood, the WPCs materials are very widely used as a wood substitute for making terraces, platforms or building facades [1]. Due to their ecological nature, the polymers from renewable resources have received considerable attention; in addition to the risks of futuristic shortages has been increased demand by the consumer society for environmentally friendly products.
It is within this framework, that biodegradable poly (lactic acid) (PLA) seems to be one of the best alternatives among all biopolymers with its promising thermal and mechanical properties as well as its low cost [5] [6] [7]. This bioplastic can be produced from renewable resources such as maize and cassava and can be biodegraded naturally into H 2 O and CO 2 [8] [9]. However, these composites have a limited number of applications because of different factors as slow crystallization kinetic, easy aging, low rigidity and high product cost. To solve these problems different types of fillers have been combined with polymer matrices to increase the thermal and mechanical properties of biocomposites [10] [11]. This work focuses on the study of Typha australis stem powder biocomposite material without the use of any kind of chemical compatibilizers. Typha australis is an aquatic plant, found on wetlands, and belongs to the family Typhaceae. It is particularly widespread in the valley of the Senegal River. This plant can reach a height of 3 meters [12] and moreover, it turns out to be harmful for agricultural production because of its invasive nature and source of pests [13]. It is used for the construction of wetlands for ecological restoration, wastewater treatment and is also the raw material for weaving paper because of its fiber length, toughness, and heat preservation performance [14] [15] [16] [17]. In this work, the morphological, thermal, rheological, and mechanical properties of biocomposites based on Typha stem powder (TSP) and Poly (lactic acid) (PLA) were studied. The relationship between the powder-mass ratio and the properties of biocomposites was analyzed.

Materials
Poly (lactic acid) (PLA) is a thermoplastic polyester produced by fermentation of renewable agricultural raw materials followed by polymerization. In this study, it has been used the PLLA (PLA4032D), which contained ~2 wt% D-lactic acid and the average molecular weight was 190,000. It was purchased by Nature Works Open Journal of Composite Materials LLC. The density, melting point (Tm) and glass transition temperature of the PLA4032D were 1.24 g/cm 3 , 170˚C, and 59.2˚C, respectively. The natural filler used was the Typha stem powder. It was collected on the Senegal River banks, in Bango in the region of Saint Louis. The plant was been cut and dried in the air then it undergoes mechanical grinding to transform the stems into powders.

Compounding and Processing
The Typha stem powder was oven-dried at 105˚C and the PLA at 60˚C for 24 hours to remove moisture. The composites were elaborated in a HAAKE Minilab twin-screw extruder (Thermo Scientific), operated at a screw speed of 100 rpm, at a temperature of 180˚C for 5 min. Four formulations of the composites were prepared with different content of filler equal to 0%, 25%, 35%, 45% in mass of TPS. The composites were then compression molded using a Carver laboratory press at 180˚C and 200 bar for 1 minute to obtain a film of about 150 µm. The film is used for the mechanical test.

Morphological Characterization
A HIROX SH4000M scanning electron microscope (SEM) was used. The samples were fractured in liquid nitrogen and after sputter-coated with gold under an argon gas flow for 15 min. The coated samples were left to dry at room temperature before SEM could be performed. The SEM analyses were done at 20 kV and at a range of magnification equal at ×80 to ×150.

Thermogravimetric Analysis (TGA)
To study the thermal degradation process of biocomposites, a TGA analysis was performed. A Mettler Toledo machine operating under a nitrogen atmosphere (20 ml/min) has been used for this purpose. The samples were analyzed at 30˚C -600˚C with a heating rate of 10˚C/min and a mass of ≈20 mg was used for each sample.

Differential Scanning Calorimetry Analysis
Thermal analysis of the biocomposite samples was carried out on a differential scanning calorimeter (METTLER TOLEDO DSC 3). All DSC measurements were performed with powdered samples of about 10 ± 0.2 mg under a nitrogen atmosphere with a flow rate of 20 ml/min. All samples were subjected to the same thermal experiment with the following thermal protocol: 1) First, the samples were heated from 25˚C to 210˚C at a heating rate of 10˚C/min to eliminate any thermal history effect; 2) Second, the samples were cooled from 210˚C to 40˚C at a cooling rate of 10˚C/min to detect the crystallization temperature (Tc); 3) Finally, the samples were heated from 25˚C to 210˚C at a heating rate of Open Journal of Composite Materials 10˚C/min to determine T m . T m and the heat of fusion (ΔH m ) were obtained from the thermograms during the second heating. The values of ΔH m were used to estimate the crystallinity degree (X c ). The degree of crystallinity (X c ) of the PLA component was determined from the following equation [16] [17]: where ΔH m , ΔH c and ΔH 0 are the heat of fusion of the composites, cold crystallization and PLA 100% crystalline, respectively. The w% TSP is the percentage of Typha stem powder. For the PLA ΔH 0 is taken to be 93 (J/g) [18].

Rheological Characterization
The viscoelastic behavior of molten polymers can be determined using oscillatory rheological experiments such as dynamic mechanical testing, which offers a convenient way to assess the frequency dependence of mechanical properties of polymers. A useful representation is to plot the experimental frequency sweep data points in the complex plane. That means that imaginary part (of the complex viscosity) η' values are reported along the abscissa (X axis) and the real ones (η'') on the ordinate (Y axis) as schematized in Figure 1; where η' is the loss viscosity, η'' is the storage viscosity and ω is the pulsation of the frequency: ω = 2πN. Usually, the experimental points are located on an arc of circle characteristic for a Cole-Cole distribution. The extrapolation of this arc of circle to the zero ordinate value gives the Newtonian viscosity which is related to the average molecular weight Mw of the considered polymer through a power law: (η 0 = K (Mw) 3.4 ) [17].
Melt rheological measurements of neat PLA and PLA composites were carried out with an ARES Rheometer Scientific mechanical spectrometer in oscillatory frequency sweep mode with a parallel-plates measuring cell. The diameter of the plates was 8 mm and the gap was 1 -1.5 mm. The frequency was ranged from 0.1 rad/s to 100 rad/s. Deformation was kept constant at 5% over the entire frequency range to ensure linearity. This strain was selected from a dynamic strain sweep test, in which, within 1% to 10% of strains, at a fixed frequency of 10 rad/s, the drift deviation from linearity was followed; the frequency sweep test was then carried out at a constant temperature at 180˚C.

Mechanical Properties
The apparatus used is a Lloyd EZ 50 traction bench. The results are analyzed using the software: NEXYGEN. The tensile strength and elongation at break of the composite were measured according to the ASTM D638-10 method at a crosshead speed of 30 mm/min. Each sample was subjected to at least 5 repetitive tests to obtain an average.

Morphological Characterization
The cross-sectional topography of PLA/TSP composites and TSP were observed by scanning electron microscopy. It can be observed from Figure 2 In addition, the presence of gaps between the pores and the two phases indicated that the motion of PLA molecules was restricted by poor interfacial compatibility [19].

Thermogravimetric Analysis
In order to better understand the effect of the TSP on the thermal degradation of the samples, thermogravimetric analysis was used. The thermogravimetric curves for all the samples are shown in Figure 3.
TSP loses moisture around 100˚C.  Figure 4 shows the thermograms corresponding to all samples, obtained from the heating and cooling cycles. The glass transition temperature (T g ) and melting temperature (T m ) of PLA were around 61˚C and 170˚C, respectively. A decrease in the cold crystallization temperature to 100˚C was noted ( Table 1)   a single peak in the biocomposites can be explained by the lowering of the mobility of PLA chains, compared with neat PLA. Moreover, this explanation is also consistent with the reduction of the temperature of cold crystallization and the increase of the degree of crystallinity (Table 1), which highlights an increase in the order of PLA chains [21]. Figure 5 represents the complex plane variations for the neat PLA and the PLA composites. As introduced above, an extrapolation of the circle arc constructed on the complex graph allows us to determine the Newtonian viscosity. Table 2 reports the Newtonian values determined for all the samples. These values show an increase in the viscosity of PLA 25TSP that is 76% higher than virgin PLA.

Rheological Behavior
Though, an increase in the quantity of the charge causes a reduction of the viscosity, reaching a Newtonian viscosity value, for the sample PLA 45TSP, comparable with that measured for PLA Pure with a difference of about 6% more.
The changing of the viscosity is caused by the perturbation of the normal polymer flow since the filler particles hinder the mobility of chain segments. Moreover, great changes are observed for the samples loaded regarding the reference Open Journal of Composite Materials  PLA Pure. All the samples with the natural fillers exhibit a deviation to the circular behavior promoting the shift of the Newtonian plateau to the low frequencies. This is characteristic of a gel behavior, indicating that at different concentrations of the powder, the level of interaction between the matrix and the filler is different at different frequencies applied [23]. In fact, at low frequencies, the viscosity strongly increases with the Typha powder content, as evidenced by the storage module of composites (G') ( Figure 6) since G' is higher than pure matrix due to the intrinsic rigidity of TSP. Shear-thinning behavior of the molten mass was observed, the viscosity of the composites is strongly influenced by the shear rate. The storage modulus, especially for the highest powder content, shows that the matrix transfers great stress to the filler and based on G' data, serving as the measure of elastic behavior, we can conclude that with the addition of the TSP the solid-like behavior for all the samples clearly increases [21].

Mechanical Properties of Biocomposites PLA/Typha Stem
The mechanical tensile properties (Young's modulus, maximum strain, ultimate tensile strength) of the biocomposites are presented in Table 3     This lowering is certainly related to the formation of aggregates and the piling up of the fibers against each other, phenomena that favor the formation of defects. At high fiber proportions, the molten mixture is very viscous and appears as "dry" and this promotes friction between fibers and contributes to the creation of pores and cavities at the interface. As a result, the fiber/matrix contact area is reduced resulting in poorer stress transfer.

Conclusion
This work has shown that the Typha stem powder can be used in PLA matrix as